Macromolecules 2009, 42, 2419-2427
1-tert-Butyl-3,3,5,5-tetraalkyl-2-piperazinon-4-oxyls: Highly Efficient Nitroxides for Controlled Radical Polymerization Saskia Miele,† Peter Nesvadba,‡ and Armido Studer*,† Institute of Organic Chemistry, Department of Chemistry, Westfa¨lische Wilhelms-UniVersita¨t Mu¨nster, Corrensstrasse 40, 48149 Mu¨nster, Germany, and Research Center Polymerization and Curing Agents, Ciba Inc., Schwarzwaldallee 215, CH-4002 Basel, Switzerland ReceiVed NoVember 19, 2008; ReVised Manuscript ReceiVed February 12, 2009
ABSTRACT: The paper describes nitroxide-mediated radical polymerization of styrene and n-butyl acrylate by using four sterically highly hindered 6-membered cyclic nitroxides. The syntheses of the corresponding alkoxyamine initiators are described, and also rate constants for C-O bond homolysis of these systems are discussed. It is shown that rate constants of alkoxyamines can readily be determined by 1H NMR experiments. Polymerization results obtained are compared with data previously achieved with highly efficient nitroxides. Since this class of nitroxides is readily accessible, the 1-tert-butyl-3,3,5,5-tetraalkyl-2-piperazinon-4-oxyl radicals bearing alkyl groups that are ethyl or larger n-alkyl groups are probably the most efficient cyclic 6-membered nitroxides known to date for mediating NMP.
Introduction Controlled living radical polymerization has received great attention during the past 10 years. Several methods that allow controlled polymerization of various monomers by radical chemistry have been developed. ATRP (atom transfer radical polymerization),1 RAFT (reversible addition-fragmentation chain transfer polymerization),2 I-group transfer polymerization,3 Te-, Sb-, and Bi-group transfer polymerization,4 cobalt-mediated polymerization,5 and NMP (nitroxide-mediated polymerization)6 are all very promising. These new methods allow the synthesis of various polymers with defined molecular weights and polydispersities below the theoretical limit (PDI < 1.5). By using either of these methods, we meanwhile reached a stage where almost every monomer can be polymerized by radical chemistry with high control. ATRP, NMP, and some cobalt-mediated polymerizations are controlled by the persistent radical effect (PRE).7,8 Importantly, in contrast to ATRP and the cobalt-mediated polymerization no metal is used in NMP.9 In the present full paper we will focus on NMP where alkoxyamines are generally used as monocomponent initiators. During polymerization dormant alkoxyamine species are reversibly formed from the corresponding nitroxides and the growing macroradical. Various nitroxides have been prepared and tested as mediators in NMP. It has been found that the structure of the nitroxide moiety heavily influences properties of a nitroxide to control the polymerization process. H-bonding,10-15 polar,16 and steric effects17-22 have been shown to alter the equilibrium constant between nitroxidecapped polymer and free nitroxide and polymer radical.16-23 A larger equilibrium constant in most of the cases leads to a more efficient polymerization.7 We showed that in cyclic 6-membered nitroxides the installation of substituents in R-position to the nitroxide N atom that are larger than methyl groups leads to “steric pressure”. The corresponding alkoxyamines such as 113 and 2a17 turned out to be highly efficient initiators/regulators for NMP (see Figure 1). However, if substituents in that position become too large (see 3),19 control of polymerization is lost. As compared to noncyclic nitroxides,24 cyclic 6-membered systems are generally more * Corresponding author. E-mail: [email protected]
† Westfa¨lische Wilhelms-Universita¨t Mu¨nster. ‡ Ciba Inc.
stable due to reversible β-elimination. For the noncyclic systems, β-elimination leads to nitroso compounds which upon leaving solvent cage generally do not reform the corresponding nitroxide. Therefore, we regard 6-membered nitroxides bearing ethyl groups in R-position to the N atom as prime candidates to control NMP. Although alkoxyamines 1 and 2 delivered excellent results, their application in NMP is hampered due to their tedious multistep synthesis. Herein we present in full details25 the synthesis of piperazinone-based alkoxyamines 4-6. Moreover, polymerization results and kinetic data will be provided. Experimental Section Materials. All reactions were performed under an argon atmosphere using the standard Schlenk technique. 1H NMR and 13 C NMR spectra were recorded on a Bruker DPX-300 (1H: 300 MHz; 13C: 75 MHz), a Varian Inova 500 (1H: 500 MHz; 13C: 125 MHz), or a Varian Unity plus 600 (1H: 600 MHz; 13C: 150 MHz). Chemical shifts δ in ppm are referenced to the solvent residual peak. Thin layer chromatography was carried out on Merck silica gel 60 F254 plates; detection by UV or dipping into a solution of KMnO4 (1.5 g), NaHCO3 (5.0 g) in H2O (400 mL), followed by heating. Flash chromatography (FC) was carried out on Merck or Fluka silica gel 60 (40 - 63 µm) at about 1.4 bar. Melting points (uncorrected) were determined on a SMP 10 apparatus (Stuart Scientific). IR spectra were recorded on a Varian 3100 FT-IR equipped with a MKII Golden Gate Single Reflection ATR unit. ESI-MS (m/z) and HRMS (m/z) were performed using a Bruker MicroTof and a Waters-Micromass Quattro LCZ (ESI-MS). Mass spectra of poly(n-butyl acrylate) before and after reinitiation for proving the livingness of the polymer chain were analyzed using the simulation software PolyCalc.26 Size exclusion chromatography (SEC) was carried out with degassed THF as eluent at a flow rate of 1.0 mL/min at rt on a system consisting of a L6200A Intelligent Pump (Merck Hitachi), a set of two PLgel 5 µm MIXED-C columns (300 × 7.5 mm, Polymer Laboratories), and a Knauer RI differential refractometer detector. Data were analyzed with PSS WinGPC Compact V.7.20 software (Polymer Standards Service) based on calibration curves built upon polystyrene and poly(methyl methacrylate) standards (Polymer Laboratories Polystyrene Medium MW Calibration Kit S-M-10 to determine the molecular weight of styrene and Poly(methyl methacrylate) Medium MW Calibration Kit M-M10 to determine the molecular weight of poly(n-butyl acrylate)) with peak molecular weights ranging from 1660 to 1 000 000 g/mol. Elemental analyses were performed on a Vario EL III (ElementarAnalysensysteme GmbH). Styrene (Acros, 99%) and n-butyl
10.1021/ma802600x CCC: $40.75 2009 American Chemical Society Published on Web 03/16/2009
2420 Miele et al. acrylate (Acros, 99%) were distilled under reduced pressure from CaH2 to remove stabilizer. Et2O was distilled from K/Na, benzene was distilled from Na, THF was distilled from K, and CH2Cl2 was distilled from P2O5. The following chemicals were purchased and used as received: acetic acid (Acros, 99.8%), ammonia solution (Acros, 25% in water), (1-bromoethyl)benzene (Alfa Aesar, 97%), 3-bromopentane (Sigma-Aldrich, 95%), chloroform (Fisher Scientific, g99%), copper powder (Sigma-Aldrich,